Kinetics of Si and Ge nanowires growth through electron beam evaporation
© Artoni et al; licensee Springer. 2011
Received: 10 September 2010
Accepted: 21 February 2011
Published: 21 February 2011
Si and Ge have the same crystalline structure, and although Si-Au and Ge-Au binary alloys are thermodynamically similar (same phase diagram, with the eutectic temperature of about 360°C), in this study, it is proved that Si and Ge nanowires (NWs) growth by electron beam evaporation occurs in very different temperature ranges and fluence regimes. In particular, it is demonstrated that Ge growth occurs just above the eutectic temperature, while Si NWs growth occurs at temperature higher than the eutectic temperature, at about 450°C. Moreover, Si NWs growth requires a higher evaporated fluence before the NWs become to be visible. These differences arise in the different kinetics behaviors of these systems. The authors investigate the microscopic growth mechanisms elucidating the contribution of the adatoms diffusion as a function of the evaporated atoms direct impingement, demonstrating that adatoms play a key role in physical vapor deposition (PVD) NWs growth. The concept of incubation fluence, which is necessary for an interpretation of NWs growth in PVD growth conditions, is highlighted.
The synthesis and the tailoring of the electrical and optical properties of nanostructured materials are fascinating research fields, and they represent a suitable route in a wide range of potential nanoscale device applications. Among these, axial structures such as C nanotubes and group IV semiconductor nanowires (NWs) are a realistic addition because of the quantum confinement of their carriers in the planar direction and because of their high surface/volume ratio. In the literature many simple device structures have been demonstrated taking advantage of the enhanced electrical properties of the NWs [1–3], of their quantum confinement for light emission [4, 5] or detection , of the decoupling of the light absorption and carrier extraction for efficient solar cell elements and of the enhanced surface effects as biochemical sensors[7, 9], or of their structure for high-performance anode batteries . A broad selection of NW composition and band structures is reported, but group IV semiconductor NWs are the most interesting at the moment because they can be easily integrated with the current CMOS technology. In particular, Si is the leading semiconductor, and its unlimited abundance makes it as the primary element for the future applications. On the other hand, Ge is experiencing a renewed interest, and it has been recently proposed for specific high-frequency applications .
Si and Ge NWs can be synthesized following a bottom-up approach, named vapor-liquid-solid (VLS) . By exploiting the self-assembling capability of the semiconductor atoms coming from the vapor phase to diffuse toward metallic droplets to form a eutectic liquid phase and, at the same time, to supersaturate the droplets performing the NWs axial growth, this approach allows the control of all the structural features of the NWs such as length, radius, and crystallographic properties. Gold has been usually chosen as a catalyst, and the influence of its diffusion on the NW sidewall has been extensively investigated . Different techniques usually benefit of the VLS mechanism. Chemical vapor deposition (CVD) has been widely used to grow NWs through the VLS mechanism. The peculiar issue of this technique is the active chemical role of the metal droplet, which catalyzes the cracking of the precursor molecule in such a way that elemental atoms are formed under the gold droplet, and the interaction with the overall substrate is quite absent.
On the contrary, the physical vapor deposition (PVD) techniques involve a different feeding contribution other than direct impingement. In fact, the metal droplet represents a thermodynamic constraint only. It determines the area in which the eutectic conditions are reached. On the other hand, the evaporated Si or Ge atoms reaching the substrate interact with the surface atoms, bond with them, and start to diffuse. They actually act as adatoms, and it is demonstrated that they play a fundamental role in the NWs growth. In particular, the microscopic growth mechanisms governing the Si and Ge NWs growth in electron beam evaporation (EBE) technique are investigated in detail. EBE is a PVD technique and, in contrast to the MBE, it is a non-ultra-high vacuum, very flexible, and economic preparation technique with broad industrial applications due to its very high potential deposition rate. In the very recent times, it has been successfully proposed for the growth of group IV semiconductor NWs because, despite its non-UHV regime, NWs synthesized by EBE have high crystallographic quality (they are single crystal and possibly faceted), and it is possible to control their length, density, as well as their crystallographic growth direction by changing the experimental parameters [14, 15].
Si and Ge have the same crystallographic structure, with a lattice misfit of about 4% only. Moreover, the Si/Au and Ge/Au phase diagrams are very similar too: each one has a single eutectic point, placed at substantially the same temperature (about 360°C), and the semiconductor percentages in the alloy at the eutectic temperature are comparable (19 and 28%, respectively) . From a thermodynamic point of view, their behavior with respect to the NW growth by VLS can be considered the same. Nevertheless, in this article, it is demonstrated that Si and Ge NWsgrowth occur in very different temperatures and fluence regimes. The growth mechanisms elucidating the relevance of the kinetic behavior of Si and Ge adatoms on the axial growth rate are investigated in detail. Finally, the contribution of the direct impingement vs the surface diffusing ad-atoms to the NWs growth in a PVD system is clarified.
Samples have been prepared in an EBE chamber which allows multiple subsequent evaporations from dissimilar and separate crucibles. Au pellets, Si ingots, or Ge ingots have been used as the sources. The evaporation flux and the nominal planar film thickness were measured in situ through a quartz microbalance. The density of these layers has been measured by comparing the thickness (measured using scanning electron microscope--SEM) with the atomic areal density (measured using Rutherford backscattering spectrometry). In contrast to Si layer, Ge layer grown by EBE shows a deeply terraced surface. Moreover, some voids are visible between terraces, and the effective density of this Ge layer is about a 20% lower than the Ge bulk density. Therefore, the evaporated flux impinging on each sample was set to the value of 2.5 × 1014 cm-2 s-1 in the case of Si and to the value of 1.5 × 1014 cm-2 s-1 in the case of Ge, to obtain the same velocity of growth of the planar films, set at a constant value of 0.05 nm s-1. The evaporated fluence has been varied in the range from 0.25 to 2.50 × 1018 atoms cm-2. The apparatus is equipped with a substrate holder which can be heated through Joule effect up to 800°C.
(111)-oriented n-type Si pieces are used as substrates in all the cases. Sample preparation procedure comprehends surface cleaning (UV oxidation followed by a dip in HF etching) to remove all surface impurities and to avoid any oxygen contamination. In fact, it has been demonstrated that the presence of the native Si oxide inhibits the NWs growth [17, 18]. Then, the samples are loaded in the vacuum chamber (base pressure of 1-2 × 10-8 mbar) where a 2-nm-thick Au layer has been first evaporated on top of the sample keeping it at room temperature. After deposition, a thermal annealing at 700°C for 2 h has been conducted to break the continuous layer and induce the formation of gold droplets on the substrate. These steps are repeated for all the samples in such a way that the substrate, the catalyst size distribution, and density are always the same. Then, Si or Ge is evaporated at the desired growth temperature, performing the NWs growth.
Structural characterization is performed using a FE-SEM Zeiss Supra 25. Plan, 65° tilted, and cross images are performed to investigate surface properties, NWs structural features, and layer thicknesses. Statistical analyses are conducted using the Gatan Digital Microscope software. Focused ion beam (FIB) experiments are performed with a 30-keV Ga+ FIB FEI V600.
Results and discussion
In the later sections of this article, the authors will elucidate the adatoms contribution by comparing the Si and Ge growth regimes. In fact, these two semiconductors have strong differences from a kinetic point of view. Despite the presence of adatoms diffusion on the substrate proceeds with the same mechanism (one of the four dangling bonds links with a dangling bond of the surface and diffusion continues till the adatom finds a more stable position where it can saturate two or more dangling bonds), and it is well known that Ge surface diffusivity on Si is very different from the self-diffusion of Si . Moreover, the melting point of Ge is 475°C lower than that of Si, and solid-phase epitaxy regrowth in Ge has a lower activation energy (E Ge = 2.0 eV) than in Si (E Si = 2.7 eV), with the same pre-exponential value (about of 3 × 108 cm s-1). As a consequence, recrystallization processes in Ge occur at much lower temperatures with respect to the typical Si temperature processes for crystalline growth [25, 26]. The differential bond energy between Si/Si and Ge/Si atoms can account for this difference, and, consequently, for the very different mobilities of these species. Moreover, according to Zakharov et al.  referring to the MBE growth technique, atoms directly impinging on the catalyst droplet allow the growth of the NWs in maintaining the Au droplet on top of it with a maximum axial rate that is equal to the planar rate. One could expect that Si or Ge NWs growth is observable in the same regime with similar structural features. On the contrary, it is shown that these two nanostructures grow at different temperatures and different fluence regimes, and these results are correlated to the different Si and Ge adatoms kinetics on the substrate.
It is intriguing to note that Si and Ge NWs growth occurs in very different regimes of temperature. In fact, Ge NWs grow, which can be observed just above the eutectic temperature (363°C). On the other hand, the minimum temperature at which Si NWs are observed is 450°C. The authors performed specific experiments at lower temperatures (360 and 420°C, respectively), but no NWs were observed in the samples. The existence of a lower bound temperature which is well above the eutectic temperature is not generally observed in some growth techniques, such as CVD growth. In fact, in the CVD technique, the semiconductor (Si or Ge) adatoms diffusion on the surface plays a minimal role with respect to direct impingement of the semiconductor gaseous species on the metallic droplet. Indeed, in PVD case it is concluded that, because of the different Si and Ge surface diffusivity, Si NWs growth needs a temperature very much higher than the Au-Si eutectic temperature, whereas Ge NWs growth is essentially limited by the eutectic temperature in such a way that thermodynamics sets a lower bound condition.
Finally, another difference arises because of the NWs length itself; while Si NWs at these conditions reach a maximum length of 200 nm, Ge NWs are taller by about a factor of 4. This evidence is strictly related to the differential axial rate behavior with respect to the temperature and the evaporated fluence of the two semiconductors; the dependence due to the latter will be discussed in the next section.
Competition between axial and 2D growth rates
Red dots and blue squares refer to the NW contributions of Si and Ge NWs, respectively. In both cases, the growth temperature of 450°C and (111)-oriented NWs only are taken into consideration, which in these growth conditions are the most observed directions. Red and blue triangles refer to the planar rate of Si and Ge layers, respectively. These values have been obtained from the cross SEM measurements of the thicknesses of the planar layers grown by evaporation, and the duration of the evaporation, by considering the different densities of Si and Ge 2D layers grown by EBE.
Differences between Si and Ge are very impressive. In fact, the axial rate of Si NWs increases only at high evaporated fluences. The minimum Si fluence necessary to observe Si NWs outside the planar layer is equal to 1.75 × 1018 cm-2. This value is defined as the incubation fluence for the growth. Moreover, after the conditions for the catalyzed growth are reached, the axial growth occurs in a limited range of evaporated fluences (from 1.75 to 2.50 × 1018 cm-2), but it is very efficient being about seven times higher than the planar rate. At the fluence value of 2.50 × 1018 cm-2, it assumes again the planar rate value. On the other hand, the behavior of Ge is very different. The incubation fluence is strongly reduced, being less than 0.25 × 1018 cm-2, i.e., the growth after evaporating a small Ge fluence is observed, which is equivalent to a planar layer of about a few nanometers. The axial rate of Ge NWs is first about seven times higher than the planar rate, and then it continuously decreases on increasing the evaporated fluence until it comes back to the planar value. The fact that the peak values of the axial rates in both Si and Ge NWs are quite similar can be attributed to the similar mechanism of surface diffusion of Si and Ge adatoms.
Direct impingement versus adatoms contribution
It is remarkable to observe that the volume ascribed to the direct impingement process on the NW growth matches very well with the volume V 2D which should be filled by the planar layer in the absence of the Au droplet. In other words, this analysis definitely demonstrates that direct impingement, in the case of PVD techniques, has a minor role in the axial growth because it contributes to a maximum NW height corresponding to the thickness of the planar layer only. NWs should not be visible outside the planar layer if direct impingement were the only mechanism for the axial growth. On the contrary, it is demonstrated that adatoms diffusion has a relevant role in the axial growth. The measured length outside the 2D film is due to this mechanism only.
On the basis of the data reported in this article, the authors have been able to model the NWs growth by PVD techniques. In particular, the differences between Si and Ge NWs behaviors will drive this modeling. In this case, the substrates are always Si wafers. When Si is evaporated, Si adatoms diffusion on Si during the whole growth process must be taken into consideration. On the contrary, at the first stages of Ge evaporation, Ge adatoms move on Si. Later, the Si from the substrate cannot interact anymore with the Ge adatoms, and they start to move on a Ge planar layer. It is reported in the literature that the diffusion mean length measured at 450°C of Ge on Si is twice greater than that of Si on Si . Moreover, the diffusion mean length of Ge on Ge is about a factor of 15 times higher than that of Si on Si. As a consequence, by changing the mean diffusion length in the different systems, the effective collecting area for the growth is changed. In particular, the collecting area for Ge NWs is much greater than for Si NWs. As a consequence, once the substrate temperature is fixed, the incubation fluence value for Ge NWs growth can be reached at lower fluence values with respect to those of the Si.
This study highlights the microscopic mechanisms occurring during the growth of Si and Ge NWs. It is demonstrated that they grow in different regimes of temperatures and fluences, despite Si and Ge having the same structure, and despite Si-Au and Ge-Au phase diagrams being very similar. First, it was proved that the minimal Si NWs growth temperature is limited by kinetics constrains. From a thermodynamic point of view, the growth could occur above 363°C. Owing to the low activation energy of the surface Si diffusion process, at temperatures less than 420°C, adatoms cannot contribute to the growth. They are substantially frozen on the substrate (i.e., their mean diffusion length is very short), and they cannot contribute to the axial growth. As a consequence, NWs are not visible outside the planar layer. On the contrary, the minimal Ge NWs growth temperature is limited by the thermodynamic constraint only (the eutectic temperature). Moreover, incubation fluences have been identified for both Si and Ge, and this value is shwon to be much higher in Si NWs than in Ge ones. Accordingly, Si NWs can grow in a very narrow fluence range at higher values than the Ge NWs. We showed that the different Si and Ge surface kinetics can well explain these differences, and we are able to model the microscopic growth mechanisms of both systems. These results open the way for an understanding of the peculiarity of the VLS mechanism in PVD systems, such as EBE to easily control the NWs growth mechanisms in achieving the maximum possible axial rate for both systems.
chemical vapor deposition
electron beam evaporation
focused ion beam
physical vapor deposition
The authors thank Carmelo Percolla for the expert technical assistance and Antonio La Mantia for FIB analyses.
- Cui Y, Zhong Z, Wang D, Wang WU, Lieber CM: High performance silicon nanowire field effect transistors. Nano Lett 2003, 3: 149. 10.1021/nl025875lView ArticleGoogle Scholar
- Zhou X, Dayeh SA, Aplin D, Wang D, Yu ET: Direct observation of ballistic and drift carrier transport regimes in InAs nanowires. Appl Phys Lett 2006, 89: 053113. 10.1063/1.2236589View ArticleGoogle Scholar
- Huang Y, Duan X, Cui Y, Lauhon LJ, Kim K, Lieber CM: Logic gates and computation from assembled nanowire building blocks. Science 2001, 294: 1313. 10.1126/science.1066192View ArticleGoogle Scholar
- Guichard AR, Barsic DN, Sharma S, Kamins TI, Brongersma ML: Tunable light emission from quantum-confined excitons in TiSi 2 -catalyzed silicon nanowires. Nano Lett 2006, 6: 2140. 10.1021/nl061287mView ArticleGoogle Scholar
- Huang MH, Mao S, Feick H, Yan H, Wu Y, Kind H, Weber E, Russo R, Yang P: Room-temperature ultraviolet nanowire nanolasers. Science 2001, 292: 1897. 10.1126/science.1060367View ArticleGoogle Scholar
- Ahn JH, Park J: Efficient visible light detection using individual germanium nanowire field effect transistors. Appl Phys Lett 2007, 91: 162102. 10.1063/1.2799253View ArticleGoogle Scholar
- Kayes BM, Atwater HA, Lewis NS: Comparison of the device physics principles of planar and radial p-n junction nanorod solar cells. J Appl Phys 2005, 97: 114302. 10.1063/1.1901835View ArticleGoogle Scholar
- Tian B, Zheng X, Kempa TJ, Fang Y, Yu N, Yu G, Huang J, Lieber CM: Coaxial silicon nanowires as solar cells and nanoelectronic power sources. Nature 2007, 449: 885. 10.1038/nature06181View ArticleGoogle Scholar
- Tian B, Kempa TJ, Lieber CM: Single nanowire photovoltaics. Chem Soc Rev 2009, 38: 16. 10.1039/b718703nView ArticleGoogle Scholar
- Chan CK, Peng H, Liu G, McIlwrath K, Zhang XF, Huggins RA, Cui Y: High-performance lithium battery anodes using silicon nanowires. Nat Nanotechnol 2008, 3: 31. 10.1038/nnano.2007.411View ArticleGoogle Scholar
- Claeys CL, Simoen E: Germanium-Based Technologies: From Materials to Devices. Oxford: Elsevier; 2007.Google Scholar
- Wagner RS, Ellis WC: Vapor-liquid-solid mechanism of single crystal growth. Appl Phys Lett 1964, 4: 89. 10.1063/1.1753975View ArticleGoogle Scholar
- Hannon JB, Kodambaka S, Ross FM, Tromp RM: The influence of the surface migration of gold on the growth of silicon nanowires. Nature 2006, 440: 69. 10.1038/nature04574View ArticleGoogle Scholar
- Irrera A, Pecora EF, Priolo F: Control of growth mechanisms and orientation in epitaxial Si nanowires grown by electron beam evaporation. Nanotechnology 2009, 20: 135601. 10.1088/0957-4484/20/13/135601View ArticleGoogle Scholar
- Pecora EF, Irrera A, Artoni P, Boninelli S, Bongiorno C, Spinella C, Priolo F: Heteroepitaxial growth and faceting of Ge nanowires on Si(111) by electron-beam evaporation. Electrochem Solid State Lett 2010, 13: K53. 10.1149/1.3339677View ArticleGoogle Scholar
- Lugstein A, Hyun YJ, Steinmar M, Dielacher B, Hauer G, Bertagnolli E: Some aspects of substrate pretreatment for epitaxial Si nanowire growth. Nanotechnology 2008, 19: 485606. 10.1088/0957-4484/19/48/485606View ArticleGoogle Scholar
- Pecora EF, Irrera A, Priolo F: Influence of O contamination and Au cluster properties on the structural features of Si nanowires. Thin Solid Films 2010, 518: 2562. 10.1016/j.tsf.2009.08.019View ArticleGoogle Scholar
- Dubrovskii VG, Sibirev NV, Harmand JC, Glas F: Growth kinetics and crystal structure of semiconductor nanowires. Phys Rev B 2008, 78: 235301. 10.1103/PhysRevB.78.235301View ArticleGoogle Scholar
- Werner P, Zakharov ND, Gerth G, Shubert L, Gosele U: On the formation of Si nanowires by molecular beam epitaxy. Int J Mater Res 2006, 97: 1008.View ArticleGoogle Scholar
- Schubert L, Werner P, Zakharov ND, Gerth G, Kolb FM, Long L, Gosele U, Tan TY: Silicon nanowhiskers grown on ⟨111⟩Si substrates by molecular-beam epitaxy. Appl Phys Lett 2004, 84: 4968. 10.1063/1.1762701View ArticleGoogle Scholar
- Sivakov V, Heyroth F, Falk F, Andra G, Christiansen S: Silicon nanowire growth by electron beam evaporation: kinetic and energetic contributions to the growth morphology. J Cryst Growth 2007, 300: 288. 10.1016/j.jcrysgro.2006.11.329View ArticleGoogle Scholar
- Sivakov V, Andra G, Gosele U, Christiansen S: Epitaxial vapor-liquid-solid growth of silicon nano-whiskers by electron beam evaporation. Phys Status Solidi A 2006, 203: 3692. 10.1002/pssa.200622156View ArticleGoogle Scholar
- Cherepanov V, Voigtlander B: Influence of material, surface reconstruction, and strain on diffusion at the Ge(111) surface. Phys Rev B 2004, 69: 125331. 10.1103/PhysRevB.69.125331View ArticleGoogle Scholar
- Csepregi L, Küllen RP, Mayer JW, Sigmon TW: Regrowth kinetics of amorphous Ge layers created by 74 Ge and 28 Si implantation of Ge crystals. Solid State Commun 1977, 21: 1019. 10.1016/0038-1098(77)90009-6View ArticleGoogle Scholar
- Olson GL, Roth J: Kinetics of solid phase crystallization in amorphous silicon. Mater Sci Rep 1988, 3: 1. 10.1016/S0920-2307(88)80005-7View ArticleGoogle Scholar
- Zakharov ND, Werner P, Gerth G, Schubert L, Sokolov L, Gosele U: Growth phenomena of Si and Si/Ge nanowires on Si (111) by molecular beam epitaxy. J Cryst Growth 2006, 290: 6. 10.1016/j.jcrysgro.2005.12.096View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.